# Electronic Supplementary Material (ESI) for Inorganic Chemistry Frontiers.
# This journal is © the Partner Organisations 2019

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_a
_database_code_depnum_ccdc_archive 'CCDC 1839687'
loop_
_audit_author_name
_audit_author_address
'D. Zhao'
;Henan Polytechnic University
China
;
_audit_update_record             
;
2018-04-26 deposited with the CCDC.	2019-11-25 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2016/6
_shelx_SHELXL_version_number     2016/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Bi K3 O13 P3 Ta'
_chemical_formula_weight         808.14

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      hexagonal
_space_group_IT_number           193
_space_group_name_H-M_alt        'P 63/m c m'
_space_group_name_Hall           '-P 6c 2'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'x-y, x, z+1/2'
'-y, x-y, z'
'-x, -y, z+1/2'
'-x+y, -x, z'
'y, -x+y, z+1/2'
'x-y, -y, -z+1/2'
'-x, -x+y, -z+1/2'
'y, x, -z+1/2'
'-y, -x, -z'
'-x+y, y, -z'
'x, x-y, -z'
'-x, -y, -z'
'-x+y, -x, -z-1/2'
'y, -x+y, -z'
'x, y, -z-1/2'
'x-y, x, -z'
'-y, x-y, -z-1/2'
'-x+y, y, z-1/2'
'x, x-y, z-1/2'
'-y, -x, z-1/2'
'y, x, z'
'x-y, -y, z'
'-x, -x+y, z'

_cell_length_a                   17.7488(15)
_cell_length_b                   17.7488(15)
_cell_length_c                   7.1137(6)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     1940.7(4)
_cell_formula_units_Z            6
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      ?
_cell_measurement_theta_max      ?

_exptl_crystal_description       ?
_exptl_crystal_colour            ?
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.149
_exptl_crystal_F_000             2172
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.100
_exptl_absorpt_coefficient_mu    23.435
_shelx_estimated_absorpt_T_min   0.089
_shelx_estimated_absorpt_T_max   0.203
_exptl_absorpt_correction_type   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  ?
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            23590
_diffrn_reflns_av_unetI/netI     0.0161
_diffrn_reflns_av_R_equivalents  0.0551
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_theta_min         2.295
_diffrn_reflns_theta_max         28.284
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             919
_reflns_number_gt                843
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+14.6457P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_extinction_coef       0.00034(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         919
_refine_ls_number_parameters     67
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0213
_refine_ls_R_factor_gt           0.0180
_refine_ls_wR_factor_ref         0.0350
_refine_ls_wR_factor_gt          0.0341
_refine_ls_goodness_of_fit_ref   1.186
_refine_ls_restrained_S_all      1.186
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
K1 K 0.40010(11) 0.28034(10) -0.250000 0.0252(4) Uani 1 2 d S T P . .
K2 K 0.666667 0.333333 0.500000 0.0280(6) Uani 1 6 d S T P . .
K3 K 0.000000 0.000000 0.000000 0.0297(9) Uani 1 12 d S T P . .
Bi1 Bi 0.22163(2) 0.22163(2) 0.250000 0.01002(9) Uani 1 4 d S T P . .
Ta1 Ta 0.500000 0.500000 0.000000 0.00884(9) Uani 1 4 d S T P . .
P1 P 0.46274(11) 0.32463(10) 0.250000 0.0118(3) Uani 1 2 d S T P . .
P2 P 0.18109(13) 0.18109(13) -0.250000 0.0119(4) Uani 1 4 d S T P . .
O1 O 0.4739(3) 0.3834(2) 0.0776(5) 0.0343(10) Uani 1 1 d . . . . .
O2 O 0.5288(3) 0.2972(3) 0.250000 0.0300(13) Uani 1 2 d S T P . .
O3 O 0.3712(3) 0.2495(3) 0.250000 0.0460(19) Uani 1 2 d S T P . .
O4 O 0.2327(3) 0.2327(3) -0.0784(7) 0.0351(13) Uani 1 2 d S T P . .
O5 O 0.1678(4) 0.0894(4) -0.250000 0.0410(15) Uani 1 2 d S T P . .
O6 O 0.5432(3) 0.5432(3) 0.250000 0.0109(12) Uani 1 4 d S T P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
K1 O3 2.597(5) 20 ?
K1 O6 2.769(5) 13_665 ?
K1 O2 2.819(5) 20 ?
K1 O1 2.845(3) 16 ?
K1 O1 2.845(3) . ?
K1 O4 2.919(4) . ?
K1 O4 2.919(4) 16 ?
K1 P1 3.227(2) 20 ?
K1 P2 3.371(3) . ?
K1 K1 3.681(3) 9_554 ?
K1 P1 3.6920(7) 1_554 ?
K1 P1 3.6921(7) . ?
K2 O2 2.827(4) 19_656 ?
K2 O2 2.827(4) 3_655 ?
K2 O2 2.827(4) 20_556 ?
K2 O2 2.827(4) 14_666 ?
K2 O2 2.827(4) 21_666 ?
K2 O2 2.827(4) . ?
K2 K2 3.5568(3) 14_667 ?
K2 K2 3.5568(3) 14_666 ?
K3 O5 3.134(5) . ?
K3 O5 3.134(5) 20_556 ?
K3 O5 3.134(5) 8_554 ?
K3 O5 3.134(5) 14 ?
K3 O5 3.134(5) 2 ?
K3 O5 3.134(5) 19_556 ?
K3 O5 3.134(5) 7_554 ?
K3 O5 3.134(5) 15 ?
K3 O5 3.134(5) 3 ?
K3 O5 3.134(5) 21_556 ?
K3 O5 3.134(5) 9_554 ?
K3 O5 3.134(5) 13 ?
Bi1 O5 2.225(5) 20_556 ?
Bi1 O5 2.225(5) 2 ?
Bi1 O4 2.345(5) . ?
Bi1 O4 2.345(5) 16_556 ?
Bi1 O3 2.445(5) 9 ?
Bi1 O3 2.445(5) . ?
Ta1 O6 1.937(2) . ?
Ta1 O6 1.937(2) 13_665 ?
Ta1 O1 1.961(3) 13_665 ?
Ta1 O1 1.961(3) 22 ?
Ta1 O1 1.961(3) 10_665 ?
Ta1 O1 1.961(3) . ?
P1 O2 1.477(5) . ?
P1 O3 1.501(5) . ?
P1 O1 1.557(3) . ?
P1 O1 1.557(3) 16_556 ?
P2 O5 1.523(6) 9_554 ?
P2 O5 1.523(6) . ?
P2 O4 1.526(5) 16 ?
P2 O4 1.526(5) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 K1 O6 171.52(15) 20 13_665 ?
O3 K1 O2 54.44(16) 20 20 ?
O6 K1 O2 117.09(14) 13_665 20 ?
O3 K1 O1 118.34(9) 20 16 ?
O6 K1 O1 58.86(8) 13_665 16 ?
O2 K1 O1 90.80(11) 20 16 ?
O3 K1 O1 118.34(9) 20 . ?
O6 K1 O1 58.87(8) 13_665 . ?
O2 K1 O1 90.80(11) 20 . ?
O1 K1 O1 109.97(16) 16 . ?
O3 K1 O4 93.73(13) 20 . ?
O6 K1 O4 93.97(11) 13_665 . ?
O2 K1 O4 140.79(11) 20 . ?
O1 K1 O4 127.12(12) 16 . ?
O1 K1 O4 85.34(13) . . ?
O3 K1 O4 93.73(13) 20 16 ?
O6 K1 O4 93.97(11) 13_665 16 ?
O2 K1 O4 140.79(11) 20 16 ?
O1 K1 O4 85.34(13) 16 16 ?
O1 K1 O4 127.12(12) . 16 ?
O4 K1 O4 49.42(19) . 16 ?
O3 K1 P1 27.21(12) 20 20 ?
O6 K1 P1 144.31(10) 13_665 20 ?
O2 K1 P1 27.22(10) 20 20 ?
O1 K1 P1 105.95(9) 16 20 ?
O1 K1 P1 105.95(9) . 20 ?
O4 K1 P1 118.17(8) . 20 ?
O4 K1 P1 118.17(8) 16 20 ?
O3 K1 P2 83.24(12) 20 . ?
O6 K1 P2 105.24(9) 13_665 . ?
O2 K1 P2 137.68(11) 20 . ?
O1 K1 P2 112.08(10) 16 . ?
O1 K1 P2 112.08(10) . . ?
O4 K1 P2 26.86(10) . . ?
O4 K1 P2 26.86(10) 16 . ?
P1 K1 P2 110.45(6) 20 . ?
O3 K1 K1 140.14(12) 20 9_554 ?
O6 K1 K1 48.33(9) 13_665 9_554 ?
O2 K1 K1 165.42(10) 20 9_554 ?
O1 K1 K1 80.91(9) 16 9_554 ?
O1 K1 K1 80.91(9) . 9_554 ?
O4 K1 K1 50.91(7) . 9_554 ?
O4 K1 K1 50.91(7) 16 9_554 ?
P1 K1 K1 167.36(4) 20 9_554 ?
P2 K1 K1 56.91(3) . 9_554 ?
O3 K1 P1 96.09(4) 20 1_554 ?
O6 K1 P1 81.88(4) 13_665 1_554 ?
O2 K1 P1 82.03(4) 20 1_554 ?
O1 K1 P1 23.26(7) 16 1_554 ?
O1 K1 P1 131.25(10) . 1_554 ?
O4 K1 P1 128.24(10) . 1_554 ?
O4 K1 P1 79.25(10) 16 1_554 ?
P1 K1 P1 88.95(4) 20 1_554 ?
P2 K1 P1 104.89(3) . 1_554 ?
K1 K1 P1 94.38(3) 9_554 1_554 ?
O3 K1 P1 96.09(4) 20 . ?
O6 K1 P1 81.88(4) 13_665 . ?
O2 K1 P1 82.03(4) 20 . ?
O1 K1 P1 131.25(10) 16 . ?
O1 K1 P1 23.26(7) . . ?
O4 K1 P1 79.25(10) . . ?
O4 K1 P1 128.24(10) 16 . ?
P1 K1 P1 88.95(4) 20 . ?
P2 K1 P1 104.89(3) . . ?
K1 K1 P1 94.38(3) 9_554 . ?
P1 K1 P1 148.89(7) 1_554 . ?
O2 K2 O2 82.90(14) 19_656 3_655 ?
O2 K2 O2 84.63(9) 19_656 20_556 ?
O2 K2 O2 112.83(18) 3_655 20_556 ?
O2 K2 O2 112.83(18) 19_656 14_666 ?
O2 K2 O2 84.63(9) 3_655 14_666 ?
O2 K2 O2 157.3(2) 20_556 14_666 ?
O2 K2 O2 84.63(9) 19_656 21_666 ?
O2 K2 O2 157.3(2) 3_655 21_666 ?
O2 K2 O2 84.63(9) 20_556 21_666 ?
O2 K2 O2 82.90(14) 14_666 21_666 ?
O2 K2 O2 157.4(2) 19_656 . ?
O2 K2 O2 84.63(9) 3_655 . ?
O2 K2 O2 82.90(15) 20_556 . ?
O2 K2 O2 84.63(9) 14_666 . ?
O2 K2 O2 112.83(18) 21_666 . ?
O2 K2 K2 51.02(6) 19_656 14_667 ?
O2 K2 K2 128.98(6) 3_655 14_667 ?
O2 K2 K2 51.02(6) 20_556 14_667 ?
O2 K2 K2 128.98(6) 14_666 14_667 ?
O2 K2 K2 51.02(6) 21_666 14_667 ?
O2 K2 K2 128.98(6) . 14_667 ?
O2 K2 K2 128.98(6) 19_656 14_666 ?
O2 K2 K2 51.02(6) 3_655 14_666 ?
O2 K2 K2 128.98(6) 20_556 14_666 ?
O2 K2 K2 51.02(6) 14_666 14_666 ?
O2 K2 K2 128.98(6) 21_666 14_666 ?
O2 K2 K2 51.02(6) . 14_666 ?
K2 K2 K2 180.0 14_667 14_666 ?
O2 K2 K1 61.38(6) 19_656 19_656 ?
O2 K2 K1 33.79(10) 3_655 19_656 ?
O2 K2 K1 129.71(10) 20_556 19_656 ?
O2 K2 K1 72.81(10) 14_666 19_656 ?
O2 K2 K1 123.78(10) 21_666 19_656 ?
O2 K2 K1 114.26(7) . 19_656 ?
K2 K2 K1 112.292(8) 14_667 19_656 ?
K2 K2 K1 67.710(8) 14_666 19_656 ?
O2 K2 K1 33.79(10) 19_656 3_656 ?
O2 K2 K1 61.38(6) 3_655 3_656 ?
O2 K2 K1 72.81(10) 20_556 3_656 ?
O2 K2 K1 129.71(10) 14_666 3_656 ?
O2 K2 K1 114.26(7) 21_666 3_656 ?
O2 K2 K1 123.78(10) . 3_656 ?
K2 K2 K1 67.709(8) 14_667 3_656 ?
K2 K2 K1 112.291(8) 14_666 3_656 ?
K1 K2 K1 58.17(3) 19_656 3_656 ?
O2 K2 K1 72.81(10) 19_656 14_666 ?
O2 K2 K1 123.78(10) 3_655 14_666 ?
O2 K2 K1 114.26(7) 20_556 14_666 ?
O2 K2 K1 61.38(6) 14_666 14_666 ?
O2 K2 K1 33.79(10) 21_666 14_666 ?
O2 K2 K1 129.71(10) . 14_666 ?
K2 K2 K1 67.710(8) 14_667 14_666 ?
K2 K2 K1 112.292(8) 14_666 14_666 ?
K1 K2 K1 91.11(3) 19_656 14_666 ?
K1 K2 K1 106.510(9) 3_656 14_666 ?
O2 K2 K1 123.78(10) 19_656 20_556 ?
O2 K2 K1 72.81(10) 3_655 20_556 ?
O2 K2 K1 61.38(6) 20_556 20_556 ?
O2 K2 K1 114.26(7) 14_666 20_556 ?
O2 K2 K1 129.71(10) 21_666 20_556 ?
O2 K2 K1 33.79(10) . 20_556 ?
K2 K2 K1 112.290(8) 14_667 20_556 ?
K2 K2 K1 67.708(8) 14_666 20_556 ?
K1 K2 K1 106.510(9) 19_656 20_556 ?
K1 K2 K1 91.11(3) 3_656 20_556 ?
K1 K2 K1 159.99(4) 14_666 20_556 ?
O5 K3 O5 69.27(13) . 20_556 ?
O5 K3 O5 110.73(13) . 8_554 ?
O5 K3 O5 180.00(18) 20_556 8_554 ?
O5 K3 O5 90.97(9) . 14 ?
O5 K3 O5 127.99(19) 20_556 14 ?
O5 K3 O5 52.01(19) 8_554 14 ?
O5 K3 O5 89.03(9) . 2 ?
O5 K3 O5 52.01(19) 20_556 2 ?
O5 K3 O5 127.99(19) 8_554 2 ?
O5 K3 O5 180.0(2) 14 2 ?
O5 K3 O5 127.99(19) . 19_556 ?
O5 K3 O5 90.97(9) 20_556 19_556 ?
O5 K3 O5 89.03(9) 8_554 19_556 ?
O5 K3 O5 134.80(19) 14 19_556 ?
O5 K3 O5 45.20(19) 2 19_556 ?
O5 K3 O5 52.01(19) . 7_554 ?
O5 K3 O5 89.03(9) 20_556 7_554 ?
O5 K3 O5 90.97(9) 8_554 7_554 ?
O5 K3 O5 45.20(19) 14 7_554 ?
O5 K3 O5 134.80(19) 2 7_554 ?
O5 K3 O5 180.00(16) 19_556 7_554 ?
O5 K3 O5 89.03(9) . 15 ?
O5 K3 O5 45.20(19) 20_556 15 ?
O5 K3 O5 134.80(19) 8_554 15 ?
O5 K3 O5 89.03(9) 14 15 ?
O5 K3 O5 90.97(9) 2 15 ?
O5 K3 O5 110.73(13) 19_556 15 ?
O5 K3 O5 69.27(13) 7_554 15 ?
O5 K3 O5 90.97(9) . 3 ?
O5 K3 O5 134.80(19) 20_556 3 ?
O5 K3 O5 45.20(19) 8_554 3 ?
O5 K3 O5 90.97(9) 14 3 ?
O5 K3 O5 89.03(9) 2 3 ?
O5 K3 O5 69.27(13) 19_556 3 ?
O5 K3 O5 110.73(13) 7_554 3 ?
O5 K3 O5 180.00(19) 15 3 ?
O5 K3 O5 134.79(19) . 21_556 ?
O5 K3 O5 90.97(9) 20_556 21_556 ?
O5 K3 O5 89.03(9) 8_554 21_556 ?
O5 K3 O5 69.27(13) 14 21_556 ?
O5 K3 O5 110.73(13) 2 21_556 ?
O5 K3 O5 90.97(9) 19_556 21_556 ?
O5 K3 O5 89.03(9) 7_554 21_556 ?
O5 K3 O5 52.01(19) 15 21_556 ?
O5 K3 O5 127.99(19) 3 21_556 ?
O5 K3 O5 45.21(19) . 9_554 ?
O5 K3 O5 89.03(9) 20_556 9_554 ?
O5 K3 O5 90.97(9) 8_554 9_554 ?
O5 K3 O5 110.73(13) 14 9_554 ?
O5 K3 O5 69.27(13) 2 9_554 ?
O5 K3 O5 89.03(9) 19_556 9_554 ?
O5 K3 O5 90.97(9) 7_554 9_554 ?
O5 K3 O5 127.99(19) 15 9_554 ?
O5 K3 O5 52.01(19) 3 9_554 ?
O5 K3 O5 180.0(2) 21_556 9_554 ?
O5 K3 O5 180.0 . 13 ?
O5 K3 O5 110.73(13) 20_556 13 ?
O5 K3 O5 69.27(13) 8_554 13 ?
O5 K3 O5 89.03(9) 14 13 ?
O5 K3 O5 90.97(9) 2 13 ?
O5 K3 O5 52.01(19) 19_556 13 ?
O5 K3 O5 127.99(19) 7_554 13 ?
O5 K3 O5 90.97(9) 15 13 ?
O5 K3 O5 89.03(9) 3 13 ?
O5 K3 O5 45.20(19) 21_556 13 ?
O5 K3 O5 134.80(19) 9_554 13 ?
O5 Bi1 O5 76.3(3) 20_556 2 ?
O5 Bi1 O4 93.77(10) 20_556 . ?
O5 Bi1 O4 93.77(10) 2 . ?
O5 Bi1 O4 93.77(10) 20_556 16_556 ?
O5 Bi1 O4 93.77(10) 2 16_556 ?
O4 Bi1 O4 170.4(3) . 16_556 ?
O5 Bi1 O3 168.2(2) 20_556 9 ?
O5 Bi1 O3 91.9(2) 2 9 ?
O4 Bi1 O3 86.92(8) . 9 ?
O4 Bi1 O3 86.92(8) 16_556 9 ?
O5 Bi1 O3 91.9(2) 20_556 . ?
O5 Bi1 O3 168.2(2) 2 . ?
O4 Bi1 O3 86.92(8) . . ?
O4 Bi1 O3 86.92(8) 16_556 . ?
O3 Bi1 O3 99.8(2) 9 . ?
O5 Bi1 K3 44.23(13) 20_556 . ?
O5 Bi1 K3 44.23(13) 2 . ?
O4 Bi1 K3 70.46(13) . . ?
O4 Bi1 K3 119.12(13) 16_556 . ?
O3 Bi1 K3 125.92(10) 9 . ?
O3 Bi1 K3 125.92(10) . . ?
O5 Bi1 K3 44.23(13) 20_556 2 ?
O5 Bi1 K3 44.23(13) 2 2 ?
O4 Bi1 K3 119.12(13) . 2 ?
O4 Bi1 K3 70.46(13) 16_556 2 ?
O3 Bi1 K3 125.92(10) 9 2 ?
O3 Bi1 K3 125.92(10) . 2 ?
K3 Bi1 K3 48.655(7) . 2 ?
O5 Bi1 K1 60.81(16) 20_556 20_556 ?
O5 Bi1 K1 137.11(16) 2 20_556 ?
O4 Bi1 K1 89.25(2) . 20_556 ?
O4 Bi1 K1 89.25(2) 16_556 20_556 ?
O3 Bi1 K1 130.96(12) 9 20_556 ?
O3 Bi1 K1 31.11(12) . 20_556 ?
K3 Bi1 K1 98.161(19) . 20_556 ?
K3 Bi1 K1 98.161(19) 2 20_556 ?
O5 Bi1 K1 137.11(16) 20_556 2 ?
O5 Bi1 K1 60.81(16) 2 2 ?
O4 Bi1 K1 89.25(2) . 2 ?
O4 Bi1 K1 89.25(2) 16_556 2 ?
O3 Bi1 K1 31.12(12) 9 2 ?
O3 Bi1 K1 130.96(12) . 2 ?
K3 Bi1 K1 98.161(19) . 2 ?
K3 Bi1 K1 98.161(19) 2 2 ?
K1 Bi1 K1 162.07(4) 20_556 2 ?
O6 Ta1 O6 180.0 . 13_665 ?
O6 Ta1 O1 90.15(15) . 13_665 ?
O6 Ta1 O1 89.85(15) 13_665 13_665 ?
O6 Ta1 O1 89.85(15) . 22 ?
O6 Ta1 O1 90.15(15) 13_665 22 ?
O1 Ta1 O1 89.6(3) 13_665 22 ?
O6 Ta1 O1 90.15(15) . 10_665 ?
O6 Ta1 O1 89.85(15) 13_665 10_665 ?
O1 Ta1 O1 90.4(3) 13_665 10_665 ?
O1 Ta1 O1 180.00(8) 22 10_665 ?
O6 Ta1 O1 89.85(15) . . ?
O6 Ta1 O1 90.15(15) 13_665 . ?
O1 Ta1 O1 180.0 13_665 . ?
O1 Ta1 O1 90.4(3) 22 . ?
O1 Ta1 O1 89.6(3) 10_665 . ?
O6 Ta1 K1 43.81(12) . 21_666 ?
O6 Ta1 K1 136.19(12) 13_665 21_666 ?
O1 Ta1 K1 89.63(12) 13_665 21_666 ?
O1 Ta1 K1 133.66(10) 22 21_666 ?
O1 Ta1 K1 46.34(10) 10_665 21_666 ?
O1 Ta1 K1 90.37(12) . 21_666 ?
O6 Ta1 K1 136.19(12) . 9_554 ?
O6 Ta1 K1 43.81(12) 13_665 9_554 ?
O1 Ta1 K1 90.37(12) 13_665 9_554 ?
O1 Ta1 K1 46.34(10) 22 9_554 ?
O1 Ta1 K1 133.66(10) 10_665 9_554 ?
O1 Ta1 K1 89.63(12) . 9_554 ?
K1 Ta1 K1 180.0 21_666 9_554 ?
O6 Ta1 K1 43.81(12) . 13_665 ?
O6 Ta1 K1 136.19(12) 13_665 13_665 ?
O1 Ta1 K1 46.34(10) 13_665 13_665 ?
O1 Ta1 K1 90.37(12) 22 13_665 ?
O1 Ta1 K1 89.63(12) 10_665 13_665 ?
O1 Ta1 K1 133.65(10) . 13_665 ?
K1 Ta1 K1 57.61(5) 21_666 13_665 ?
K1 Ta1 K1 122.39(5) 9_554 13_665 ?
O6 Ta1 K1 136.19(12) . . ?
O6 Ta1 K1 43.81(12) 13_665 . ?
O1 Ta1 K1 133.66(10) 13_665 . ?
O1 Ta1 K1 89.63(12) 22 . ?
O1 Ta1 K1 90.37(12) 10_665 . ?
O1 Ta1 K1 46.35(10) . . ?
K1 Ta1 K1 122.39(5) 21_666 . ?
K1 Ta1 K1 57.61(5) 9_554 . ?
K1 Ta1 K1 180.0 13_665 . ?
O2 P1 O3 113.1(3) . . ?
O2 P1 O1 111.4(2) . . ?
O3 P1 O1 108.3(2) . . ?
O2 P1 O1 111.4(2) . 16_556 ?
O3 P1 O1 108.3(2) . 16_556 ?
O1 P1 O1 103.9(3) . 16_556 ?
O2 P1 K1 60.8(2) . 20_556 ?
O3 P1 K1 52.3(2) . 20_556 ?
O1 P1 K1 127.70(13) . 20_556 ?
O1 P1 K1 127.70(13) 16_556 20_556 ?
O2 P1 K1 97.70(6) . 1_556 ?
O3 P1 K1 74.56(3) . 1_556 ?
O1 P1 K1 145.63(16) . 1_556 ?
O1 P1 K1 46.19(13) 16_556 1_556 ?
K1 P1 K1 82.11(4) 20_556 1_556 ?
O2 P1 K1 97.70(6) . . ?
O3 P1 K1 74.56(3) . . ?
O1 P1 K1 46.19(13) . . ?
O1 P1 K1 145.63(16) 16_556 . ?
K1 P1 K1 82.11(4) 20_556 . ?
K1 P1 K1 148.89(7) 1_556 . ?
O5 P2 O5 104.5(5) 9_554 . ?
O5 P2 O4 111.54(16) 9_554 16 ?
O5 P2 O4 111.54(16) . 16 ?
O5 P2 O4 111.54(16) 9_554 . ?
O5 P2 O4 111.54(16) . . ?
O4 P2 O4 106.3(4) 16 . ?
O5 P2 K1 160.8(3) 9_554 . ?
O5 P2 K1 94.6(2) . . ?
O4 P2 K1 59.82(16) 16 . ?
O4 P2 K1 59.82(16) . . ?
O5 P2 K1 94.6(2) 9_554 9_554 ?
O5 P2 K1 160.8(3) . 9_554 ?
O4 P2 K1 59.82(16) 16 9_554 ?
O4 P2 K1 59.82(16) . 9_554 ?
K1 P2 K1 66.19(7) . 9_554 ?
O5 P2 K3 57.6(2) 9_554 2_554 ?
O5 P2 K3 57.6(2) . 2_554 ?
O4 P2 K3 97.9(2) 16 2_554 ?
O4 P2 K3 155.8(2) . 2_554 ?
K1 P2 K3 137.142(19) . 2_554 ?
K1 P2 K3 137.143(19) 9_554 2_554 ?
O5 P2 K3 57.6(2) 9_554 . ?
O5 P2 K3 57.6(2) . . ?
O4 P2 K3 155.8(2) 16 . ?
O4 P2 K3 97.9(2) . . ?
K1 P2 K3 137.142(19) . . ?
K1 P2 K3 137.143(19) 9_554 . ?
K3 P2 K3 57.91(4) 2_554 . ?
P1 O1 Ta1 144.4(2) . . ?
P1 O1 K1 110.55(17) . . ?
Ta1 O1 K1 103.75(14) . . ?
P1 O2 K1 92.0(2) . 20_556 ?
P1 O2 K2 131.67(16) . 14_666 ?
K1 O2 K2 112.29(14) 20_556 14_666 ?
P1 O2 K2 131.67(16) . . ?
K1 O2 K2 112.30(14) 20_556 . ?
K2 O2 K2 77.96(13) 14_666 . ?
P1 O3 Bi1 139.7(3) . . ?
P1 O3 K1 100.5(3) . 20_556 ?
Bi1 O3 K1 119.8(2) . 20_556 ?
P2 O4 Bi1 138.3(3) . . ?
P2 O4 K1 93.32(19) . . ?
Bi1 O4 K1 118.11(15) . . ?
P2 O4 K1 93.32(19) . 9_554 ?
Bi1 O4 K1 118.11(15) . 9_554 ?
K1 O4 K1 78.18(14) . 9_554 ?
P2 O5 Bi1 150.4(4) . 15 ?
P2 O5 K3 98.1(2) . 2_554 ?
Bi1 O5 K3 106.10(18) 15 2_554 ?
P2 O5 K3 98.1(2) . . ?
Bi1 O5 K3 106.10(18) 15 . ?
K3 O5 K3 69.15(13) 2_554 . ?
Ta1 O6 Ta1 133.3(3) . 4_665 ?
Ta1 O6 K1 107.22(9) . 21_666 ?
Ta1 O6 K1 107.22(9) 4_665 21_666 ?
Ta1 O6 K1 107.22(9) . 13_665 ?
Ta1 O6 K1 107.22(9) 4_665 13_665 ?
K1 O6 K1 83.34(17) 21_666 13_665 ?

_refine_diff_density_max         0.716
_refine_diff_density_min         -0.833
_refine_diff_density_rms         0.160



